doi:10.4236/msa.2011.210195 Published Online October 2011 (http://www.SciRP.org/journal/msa)
Effect of Laser Beam Welding Parameters on
Microstructure and Properties of Duplex
Abdel-Monem El-Batahgy1, Abdel-Fattah Khourshid2, Thoria Sharef2
1Manufacturing Technology Department, Central Metallurgical Research and Development Institute, Cairo, Egypt; 2Mechanical De-sign and Production Department, Faculty of Engineering, Tanta University, Tanta, Egypt.
Received June 26th, 2011; revised July 19th, 2011; accepted August 25th, 2011.
The present study is concerned with laser beam welding and its effect on size and microstructure of fusion zone then, on mechanical and corrosion properties of duplex stainless steel welded joints. In this regard, influence of different laser welding parameters was clarified. Both bead-on-plate and autogenously butt welded joints were made using carbon dioxide laser with a maximum output of 9 kW in the continuous wave mode. Welded joints were subjected to visual, dye penetrant and radiography tests before sectioning it for different destructive tests. Accelerated corrosion test was car-ried out based on tafel plot technique. The results achieved in this investigation disclosed that welding parameters play an important role in obtaining satisfactory properties of welded joint. High laser power and/or high welding speed to-gether with adjusting laser focused spot at specimen surface have produced welded joints with a remarkable decrease in fusion zone size and an acceptable weld profile with higher weld depth/width ratio. Besides, acceptable mechanical and corrosion properties were obtained. Using nitrogen as a shielding gas has resulted in improving mechanical and corrosion properties of welded joints in comparison with argon shielding. This is related to maintaining proper fer-rite/austenite balance in both weld metal and HAZ in case of nitrogen shielding. As a conclusion, laser power, welding speed, defocusing distance and type of shielding gas combination have to be optimized for obtaining welded joints with acceptable profile as well as mechanical and corrosion properties.
Keywords: Duplex Stainless Steel, Laser Beam Welding, Laser Power, Welding Speed, Defocusing Distance, Shielding
Gas Type, Fusion Zone, Microstructure, Mechanical Properties, Corrosion Resistance
The duplex stainless steels have been developed to pro-vide a combination of strength and resistance to pitting and stress corrosion cracking in comparison with the 300-series austenitic stainless steels [1-3]. These unique properties of the duplex stainless steels have resulted in their use in a variety of industrial applications, including chemical process plant piping, oil and gas transmission lines, and structures for use in marine environments [4,5]. Since welding is widely used in these applications, un-derstanding the factors which affect the weldability of duplex stainless steels is critical to the successful imple-mentation of these engineering materials.
Generally, the ferrite/austenite balance has a remark-able influence on both mechanical and corrosion
ties of duplex stainless steels [6,7]. The optimum proper-ties of duplex stainless steels are achieved when nearly equal proportions of austenite and ferrite are present in the microstructure. In base metals, this phase balance is obtained by an appropriate combination of composition and solution heat treatment. However, control of the fer-rite/austenite balance in welds is not as straightforward as in the base metals [8-11].
welding parameters on properties of duplex stainless steels. The present study is concerned with laser beam welding and its effect on size and microstructure of fu-sion zone then, on mechanical and corrofu-sion properties of duplex stainless steel welded joints.
2. Experimental Procedure
The used steel is a commercial duplex stainless steel; 2205 with 6.4 mm plate thickness. Its chemical composi-tion and mechanical properties are given in Table 1. Both bead-on-plate and autogenously single pass square butt welds were made using CO2 laser beam welding
process. Schematic illustration of laser butt welding joint is shown in Figure 1. Weld specimens (150 × 100 × 6.4 mm) were prepared as square butt joints with machined surfaces and were held firmly using fixture to prevent distortion. Laser beam welding parameters studied are given in Table 2.
The used laser was a carbon dioxide with a maximum output power of 9 kW in the continuous wave mode. Af-ter welding, the specimens were visually inspected, ra-diographed then, sectioned transverse to the welding di-rection where it were subjected to metallographic ex-aminations as well as mechanical and corrosion tests. For metallographic examination, the specimens were pre-pared using standard techniques. The size and micro-structure of fusion zone were examined using optical microscope. Compositional variations across welded joints were determined in scanning electron microscope equipped with an energy dispersive spectrometer (EDS) at an accelerating voltage of 30 kV. The elements ana-
lyzed included both ferrite and austenite stabilizing ele-ments.
Mechanical tests including tensile, bending and hard-ness were performed for laser beam butt welded joints having complete penetration. These tests were performed at room temperature according to relevant standards. Tensile test was performed for three samples in each condition and the data reported are the average of the three individual results. The given hardness values are the average of five readings. Regarding corrosion test, selected laser beam welded samples were subjected to accelerated corrosion test based on tafel plot technique where corrosion rate was measured using Potentio-stat—Auto Lab PGSTAT 30 device.
3. Results and Discussion3.1. Effect of Laser Power
The effect of laser power was clarified using 0.5m/min welding speed, 0.0 and −2.0 mm defocusing distances.
Figure 2 shows macrographs of cross sections of laser bead-on-plate welds made using 0.5 m/min welding
Figure 1. Schematic illustration of laser butt welding joint.
Table 1. Chemical composition (wt%) and mechanical properties of used base metal.
Cr Ni Mn C Si P S Mo Cu N
21.9 4.70 1.71 0.03 0.50 0.03 0.002 2.60 0.20 0.17
Tensile strength (MPa) Yield strength (MPa) Elongation (%)
730 685 30
Table 2. Laser beam welding parameters.
Weld type P (kW) S (m/min) △Z (mm) Shielding gas/ Flow rate (l/min)
Bead-on-plate 4, 5, 6, 7, 7.5, 8 0.5 −2, 0 Argon/20
Bead-on-plate 7 0.25, 0.4, 0.5, 1, 2, 3, 4, 5, 6 −2, 0 Argon/20
Bead-on-plate 7 0.5 3, 2, 1, 0, −1, −2, −3, −4 Argon/20
Butt joint 8 0.25, 0.5 −2 Nitrogen/20
Figure 2. Macrographs of cross sections of laser bead-on-plate welds made using 0.5 m/min speed, −2 mm defocusing dis-tance, 20 l/min Ar and different laser powers. (a) 4 kW; (b) 5 kW; (c) 7 kW; (d) 8 kW.
speed, −2 mm defocusing distance, 20 l/min Ar and dif-ferent laser powers. It is clear that penetration depth in-creases with increasing laser power. The weld bead showed a characteristic of laser welding where the de-velopment of the weld is essentially symmetrical about the axis of the laser beam. No welding cracks or porosity were found and this could be partly due to the good crack resistance of the base metal and the welding conditions provided. Figure 3 summarizes the results of penetration depth measurements as a function of laser power. It can be noticed that penetration depth is sharply increasing with the increase of laser power. It increased from 3.4mm to 4.7mm with increasing power from 4 to 8 kW.
3.2. Effect of Laser Welding Speed
Macrographs of cross sections of laser bead-on-plate welds made using 8 kW laser power, –2 mm defocusing distance, 20 l/min Ar and different welding speeds are shown in Figure 4. It is noteworthy that the fusion zone is symmetrical about the axis of the laser beam. However, size and depth/width ratio of fusion zone are significantly affected by welding speed. A lower welding speed re-sulted in a remarkable increase in the fusion zone size. Also, weld depth/width ratio was remarkably increased with decreasing welding speed. Consequently, acceptable weld profile was obtained where the fusion zone inter-face is a smooth curve with no inflections. Complete penetration with relatively acceptable fusion zone size for the 6.4 mm base metal thickness was obtained at welding speed of 0.25 m/min (Figure 4(d)). In other words, 0.25 m/min is considered as the optimum welding speed at 8kW laser power since it resulted in fusion zone with a slight taper configuration. This fusion zone shows a characteristic of laser welding with an acceptable weld depth/width ratio. At low welding speed, attenuation of beam energy by plasma is less significant. This results in relatively more exposure of the laser beam on the sample surface. Consequently, the depth/width ratio would be decreased and the fusion zone would be increased.
Inspite of the development of the weld is essentially symmetrical about the axis of the laser beam, increase
0.5m/min, -2.0mm, 20l/min Ar
2 2.5 3 3.5 4 4.5 5
3 4 5 6 7 8
Figure 3. Effect of laser power on weld depth of laser bead- on-plate welds made using 0.5 m/min speed and −2 mm defocusing distance and 20 l/min Ar shielding.
penetration at the root side was observed particularly at lower welding speed suggesting an unsteady fluid flow. This is due to the presence of two strong and opposing forces, namely, the electromagnetic and the surface ten-sion gradient forces. At these locations, the electromag-netic force may have overcome the surface tension force, thereby, influencing convective heat transfer. As a result, any local perturbation in the over weld can cause the flow field to change dramatically, resulting in the ob-served increased penetration.
It can be noticed that no welding cracks or porosity were found and this could be partly due to the good crack resistance of base metal and the welding conditions pro-vided. Figure 5 summarizes the results of weld depth measurements as a function of welding speed. Weld depth is decreased with the increase in welding speed. It decreased from 7.4mm to 1.9mm with increasing weld-ing speed from 0.25 to 6 m/min.
3.3. Effect of Defocusing Distance
Defocusing distance, focus position, is the distance be-tween specimen surface and optical focal point. In order to study its effect on both penetration depth and weld profile, bead-on-plate was made with changing defocus-ing distance of −4.0 mm up to 3.0 mm. Welding condi-tions were selected to obtain incomplete penetration.
Figure 4. Macrographs of cross sections of laser bead-on-plate welds made using 8 kW laser power, –2 mm defocusing dis-tance, 20 l/min Ar and different welding speeds. (a) 5 m/min; (b) 1 m/min; (c) 0.5 m/min; (d) 0.25 m/min.
8kW, 0.0mm, 20l/min Ar
0 2 4 6 8 10
0 1 2 3 4 5 6 7
Figure 5. Effect of welding speed on weld depth of laser bead-on-plate welds made using 8 kW power, −2 mm defo-cusing distance and 20 l/min Ar shielding.
Examples of macrographs of cross sections of laser bead-on-plate welds made using 8 kW power, 0.5 m/min welding speed, 20 l/min argon shielding and different defocusing distances are shown in Figure 6. No cracking or porosity was observed in all welds. Figure 7 summa-rizes results of weld bead depth/width ratio as a function of defocused distance of laser bead-on-plate welds made using 8 kW power, 0.5 m/min welding speed and 20 l/min Ar. Changing defocusing distance from zero to either minus or plus values has resulted in decrease in depth/ width ratio. In other words, shifting the focused beam position to either below or above specimen surface re-sults in decrease in depth/width ratio. However, shifting the focused beam position above the specimen surface results in much decrease in depth/width ratio in com-parison with shifting it below specimen surface. This is related to decrease in laser beam density in case of shift-ing the focused beam position above specimen surface. The above results are in good agreement with other re-search work .
3.4. Effect of Type of Shielding Gas
Based on results obtained from above experiments, op-timum welding parameters were obtained and imple-mented for welding square butt joints. Nondestructive investigations including visual, dye penetrant and
radio-graphic tests confirmed that laser butt welded joint is free from both external and internal defects. Then, welded joint was sectioned for metallographic examinations.
Figure 8(a) shows macrograph of a cross section of laser butt welded joints made using 8 kW power, 0.5 m/min speed, 0.0mm defocusing distance and 20 l/min argon. Fusion zone shows a characteristic of laser welding with complete penetration and acceptable weld profile where the fusion zone interface is a smooth curve with no in-flections.
In order to clarify the effect of shielding gas type, ar-gon was replaced by nitrogen with other welding condi-tions kept constant. Figure 8(b) shows macrograph of a cross section of laser butt welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min nitrogen. It can be noticed that typical laser weld with complete penetration and acceptable weld pro-file, similar to that of argon shielding, was obtained.
3.5. Microstructure of Laser Butt Welds
The microstructure of the used 2205 duplex stainless steel base metal is shown in Figure 9. It can be noticed that this microstructure is duplex with approximately equal volumes of both ferrite and austenite phases. Since hot working of duplex stainless steel is normally per-formed in the austenite-ferrite, two phase region, the re-sultant microstructure tends to be strongly oriented along the working direction. An average hardness value of about 305 Hv was obtained for this microstructure.
Optical micrographs of laser butt welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min of argon and nitrogen shielding are shown in Figures 10 and 11 respectively. The noticeable feature is the highly directional nature of the microstruc-ture around the axis of the laser beam in both cases. This is due to solidification of the weld metal at high cooling rate. No solidification cracking was found in the weld structure. Structures of weld metal in both joints were almost similar. For weld metal, a dendritic microstructure was developed at fusion boundary due to fast cooling conditions (Figures 10(c), 11(c)). More globular struc-tures were observed at weld metal center that exposed to
(a) (b) 2mm (c) 2mm
Figure 6. Macrographs of cross sections of laser bead-on-plate welds made using 8 kW power, 0.5 m/min speed, 20 l/min Ar with difference defocusing distances. (a) Dd = −4 mm; (b) Dd = −1 mm; (c) Dd = 0.0 mm; (d) Dd = +3 mm.
0 0.2 0.4 0.6 0.8 1 1.2
Defocusing Distance, mm
Figure 7. Weld bead depth/width ratio versus defocusing distance of laser bead-on-plate welds made using 8 kW power, 0.5 m/min speed and 20 l/min Ar.
Figure 8. Macrographs of cross sections of laser butt welded joints made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min of (a) argon; (b) nitrogen.
lower cooling rates and with a less pronounced heat flow direction. During solidification of duplex weld metal an almost completely ferrite structure is formed. Further cooling initiates the formation of the austenite phase nu-cleating at the ferrite grain boundaries. In other words, duplex stainless steel weld metal solidifies completely to
α-ferrite and the volume fraction of austenite is deter-mined by subsequent solid state phase transformation (17).
Figure 9. Optical micrographs of base metal of duplex stain- less steel used.
Regarding heat affected zone, its microstructure is critical for welded joint properties. In general, narrow HAZ of about 400 - 500 µm was observed for the exam-ined welds (Figures 10(a), 11(a)). The heat affected zone is consisting firstly of a grain growth zone charac-terized by coarse α-ferrite grains decorated with al-lotriomorphic layers of austenite, some austenite plates and some intra-granularly nucleated particles formed on inclusions where the volume fraction of austenite in this region is low compared with the base metal. Beyond this partially ferritised zone, the major difference being the spacing of the grains which is a function of the distance from the fusion zone and the peak temperature reached during heating. In other words, the coarse grained region adjacent to the fusion line could be resulted from nearly complete austenite dissolution on heating and subsequent ferrite grain growth. Higher magnifications for HAZ mi-crostructure are shown in color etching in Figure 12 and hardness measurements allowed a clear distinction be-tween the ferrite and austenite in both weld metal and HAZ. The ferrite content in both weld metal and HAZ was relatively higher in comparison to base metal. This has been confirmed using energy dispersive X-ray (EDX) technique. Results showed that the concentrations of elements; such as Cr and Mn in ferrite phase is higher, while Ni concentration is lower than in austenitic phase. The element partitioning between ferritic and austenitic phase is consistent with the stabilizing effect of each
Figure 10. Optical micrographs of laser butt welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing dis-tance and 20 l/min argon shielding.
Figure 11. Optical micrographs of laser butt welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing dis-tance and 20 l/min nitrogen shielding.
100 µm WM
100 µm WM
Figure 12. Color etched optical micrographs of HAZ of laser butt welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min of (a) argon shielding; (b) nitrogen shielding.
element on the respective phase.
Generally, laser weld results in a rapid cooling rate through the transformation temperature range which in turn resulted in decreasing austenite content and this agreed qualitatively with optical metallography. Variation
in ferrite/austenite balance among different heat input of laser welds can be rationalized using a constant iron sec-tion of a Fe-Cr-Ni ternary phase diagram. The composisec-tion band superimposed on the 60% constant iron section is representative of the range of duplex stainless steel con-sidered in this investigation. The diagram predicts that primary solidification of this alloy occurs as delta ferrite and that the structure is completely ferritic at completion of solidification. On cooling in the solid state, partial trans-formation of ferrite to austenite occurs at temperatures below the ferrite solves. The austenite content formed during cooling in solid state is depended on cooling rate. The higher the laser power and/or the lower welding speed, the coarser is the dendritic structure due to decreasing cooling rate. However, the effect of laser power was rela-tively less than that of welding speed.
3.6. Mechanical Properties of Laser Butt Welds
Hardness profile through weld metal, HAZ and base metal of welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min argon is shown in Figure 13. It can be noticed that no significant difference in hardness values of weld metal, HAZ and base metal was obtained. Similar hardness pro-file was obtained in case of nitrogen shielding.
The bending test at room temperature showed good ductility for all joints where no cracks were found after U-bends made. Results of tensile test of laser butt welded joint, made using 8 kW power, 0.5 m/min speed, 0.0 mm
400 µm BM
100 µm BM
(c) 50 µm
400 µm BM
100 µm BM
(c) 50 µm
200 250 300 350
0 1 2 3 4 5
Distance from Weld Centerline, mm
WM HAZ BM
Figure 13. Hardness profile through weld metal, HAZ and base metal of welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min ar-gon.
defocusing distance and 20 l/min argon, as well as that of base metal are shown in Table 3. Tensile tested welded specimens were failed outside weld zone. Tensile proper-ties of welded specimens are very close to that of base metal. Only, ductility or elongation of welded joint is slightly lower than that of base metal. This is related to decreasing austenite volume fraction of welded joint in comparison with base metal.
The obtained mechanical properties, in general, are correlated to microstructure that was affected by shield-ing gas type. In other words, mechanical properties of welds made using nitrogen shielding are relatively im-proved in comparison with that of welds made using ar-gon shielding. This could be related to better balancing of ferrite-austenite phases in both weld metal and heat affected zone since nitrogen is austenite stabilizer and is of great importance in the reforming of austenite that in turn could result in structure with approximately equal amounts of ferrite and austenite, similar to that of base metal. This is conformed to results of other researchers’ work .
It should be reported that tensile elongation of laser welded joint was not remarkably affected by increasing heat input as a function of higher laser power and/or lower welding speed inspite of higher austenite volume fraction in this case. This could be related to larger fusion zone size in case of higher heat input. In other words, the effect of fusion zone size to decrease tensile elongation is higher than the effect of austenite volume fraction to in- crease it.
Table 3. Tensile properties of laser butt welded joint made using 8 kW power, 0.5 m/min speed, 0.0 mm defocusing distance and 20 l/min argon, as well as that of base metal.
specimen Tensile strength (MPa) Yield strength (MPa) Elongation (%)
Welded joint 713 669 25
Base metal 730 685 30
3.7. Corrosion Properties of Laser Butt Welds
The effect of both heat input, as a function of welding speed, and shielding gas type on corrosion resistance of laser butt welded joints are shown in Table 4 and Figure 14. It is found that corrosion rate of welded joint de-creases with the increase in welding speed that means with the decrease in heat input. This effect of heat input can be rationalized in terms of cooling rate. For the low heat input of laser welds, the fast cooling rate resulted in insufficient amount of austenite and significant chro-mium nitride precipitation. This could lead to depletion of chromium around these precipitates which in turn could have a deleterious effect on the pitting resistance. It is found also that using nitrogen as a shielding gas to replace argon, under same flow condition, has resulted in a remarkable decrease in corrosion rate of welded joint (Figure 14). Again, improvement in corrosion properties of laser beam welded joints made using nitrogen as a shielding gas is related to improvement in ferrite-auste- nite balance in both weld metal and heat affected zone, as has been reported by other research works [19,20].
Based on the results achieved in this study, it can be con-cluded that laser power, welding speed, defocusing dis-tance and type of shielding gas combinations have to be optimized for obtaining welded joints with acceptable fusion zone size, weld profile as well as mechanical and corrosion properties.
The minimum fusion zone produced by laser beam is depended on heat input as a function of laser power and welding speed. High laser power and high welding speed together with adjusting laser focused spot at specimen surface have produced welded joint with a remarkable decrease in fusion zone size and an acceptable weld profile
Table 4. Corrosion rate of laser beam welded joints made using different welding speeds and different shielding gases.
Welding condition Corrosion rate, mm/year Remarks
8 kW, 0.5 m/min, 20 l/min, Nitrogen 0.001637 Weld metal-fusion line corrosion
8 kW, 0.5 m/min, 20 l/min Argon 0.05334 Weld metal-fusion line corrosion
Figure 14. Comparison between corrosion rate of laser beam welded joints made using different welding speeds and shielding gases.
with higher weld depth/width ratio. The nature of ferrite to austenite transformation in fusion zone is strongly influ-enced by cooling rate, which is depended on heat input as a function of laser power and/or welding speed. Low heat input laser welds resulted in considerable variation in the ferrite/austenite balance of fusion zone relative to the base metal as a result of high cooling rate.
Satisfactory mechanical properties including yield strength, tensile strength, elongation and bending were obtained for laser welds. Results indicated that heat input has no remarkable effect on mechanical properties, ex-cept elongation that was improved with either increasing laser power or decreasing welding speed that means with increasing heat input. This is related to maintaining pro- per ferrite-austenite balance in fusion zone in this case. Using nitrogen to replace argon as a shielding gas, under same flow rate, has resulted in remarkable decrease in corrosion rate and increase in ductility of welded joint. Improvement in both mechanical and corrosion proper-ties of laser beam welded joints made using nitrogen as a shielding gas is related to maintaining proper ferrite- austenite balance in both weld metal and heat affected zone.
The authors would like to acknowledge Libyan Research Institute for conducting laser beam welding experiments.
 B. I. Voronenko, “Austenitic-Ferritic Stainless Steels: A State-of-the Art Review,” Metal Science and Heat Treat-ment, Vol. 39, No. 9-10, 1997, pp. 428-437.
 A. Poznansky, C. S. Nalbone and J. D. Crawford, “The Corrosion Resistance of 25Cr-3.5Mo-6Ni and 25Cr 4.5Mo- 6Ni Cast Duplex Stainless Steels,” Proceedings of Inter-national Conference, Duplex Stainless Steels, St. Louis, 25-28 October 1983, pp. 431-444.
 N. Lopez, M. Cid and M. Puigalli, “Influence of σ-Phase on Mechanical Properties and Corrosion Resistance of Duplex Steels,” Corrosion Science, Vol. 41, No. 8, 1999, pp. 1615-1631. doi:10.1016/S0010-938X(99)00009-8
 M. Tynell, “Applicability Range for a High Strength Du-plex Stainless Steel in Deep Sour Oil and Gas Wells,”
Proceedings of International Conference, Duplex Stain- less Steels, St. Louis, 25-28 October 1983, pp. 283-292.  H. Miyuki, T. Kudo, M. Koso, M. Miura and T. Moroishi,
“25%Cr Containing Duplex Phase Stainless Steel for Hot Sea Water Applications,” Proceedings of International Conference, Duplex Stainless Steels, St. Louis, 25-28 October 1983, pp. 95-112.
 S. M. Tavares, V. F. Terra, J. M. Pardal and M. P. Fon- seca, “Influence of the Microstructure on the Toughness of a Duplex Stainless Steel UNS S31803,” Journal of Materials Science, Vol. 40, No. 1, 2005, pp. 145-154.
 L. F. Svensson and B. Gretoft, “Properties-Microstructure Relationship for Duplex Stainless Steel Weld Metals,”
Proceedings of International Conference, Duplex Stainless Steel, The Hague, 27-28 October 1986, Paper 22.
 M. Miura, T. Kudo, M. Tsuge, M. Kuso and T. Kobaya-shi, “Effect of Chemical Composition on Microstructure, Mechanical and Corrosion Properties of Duplex Stainless Steel Weldment,” Proceedings of International Confer-ence, Duplex Stainless Steel, The Hague, 27-28 October 1986, paper 33C.
of Duplex Stainless Steel Weldments,” Materials Science Forum, Vol. 561-565, 2007, pp. 2119-2122.
 V. Muthupandi, P. B. Srinivasan, S. K. Seshadri and S. Sundaresan, “Effect of Weld Metal Chemistry and Heat Input on the Structure and Properties of Duplex Stainless Steels,” Materials Science Engineering: A, Vol. 358, No. 1-2, 2003, pp. 9-16. doi:10.1016/S0921-5093(03)00077-7
 J. Honeycombe and T. G. Gooch, “Intergranular Attack in Welded Stress-Corrosion Resistant Stainless Steels,” Weld- ing Journal, Vol. 56, No. 11, 1977, pp. 339-s-353-s.  R. Mundt and H. Hoffmeister, “Effect of Chemical
Com-position and Weld Thermal Cycles on Phase Transforma-tion and Microstructures of Ferrite-Austenite Steels,”
Proceedings of International Conference, Stainless Steel, Gothenberg, 3-4 September 1984, pp. 315-322.
 S. Jana, “Effect of Heat Input on HAZ Properties of Two Duplex Stainless Steels,” Journal of Materials Processing Technology, Vol. 33, No. 3, 1992, pp. 247-261.
 B. Bonnefois, R. Blondeau and D. Catelin, “Control of the Ferrite Level in Duplex Stainless Steel Welds,” Pro-ceedings of International Conference, Duplex Stainless Steel, The Hague, 27-28 October 1986, Paper 6.
 J. Ku, N. Ho and S. Tjong, “Properties of Electron Beam Welded SAF 2205 Duplex Stainless Steel,” Journal of Materials Processing Technology, Vol. 63, No. 1-3, 1993,
pp. 770-775. doi:10.1016/S0924-0136(96)02721-5
 A. El-Batahgy, “Effect of Laser Beam Welding Parame-ters on Fusion Zone Shape and Microstructure of Austen-itic Stainless Steel,” Materials Letters, Vol. 32, No. 2-3, 1997, pp. 155-163. doi:10.1016/S0167-577X(97)00023-2
 J. Nowacki and A. Lukojc, “Microstructural Transforma-tions of Heat Affected Zones in Duplex Steel Welded Joints,” Materials Characterization, Vol. 56, No. 4-5, 2006, pp. 436-441. doi:10.1016/j.matchar.2006.02.007
 T. Omura, T. Kushida and Y. Komizo, “Effect of Nitro-gen Distribution on Rapid Solidification in Laser Welded Duplex Stainless Steels,” Welding International, Vol. 14, No. 4, 2000, pp. 288-294.
 P. Bala Srinivasan, V. Muthupandi, W. Dietzel and V. Sivan, “Microstructure and Corrosion Behavior of Shield- ed Metal Arc Welded Dissimilar Joints Comprising Du- plex Stainless Steel and Low Alloy Steel,” Materials En- gineering and Performance, Vol. 15, No. 6, 2006, p. 758.
 G. Lothongkum, P. Wongpanya, S. Morito, T. Furuhara and T. Maki, “Effect of Nitrogen on Corrosion Behaviour of 28Cr-7Ni Duplex and Microduplex Stainless Steels in Air-Saturated 3.5 wt% NaCl Solution,” Corrosion Sci-ence, Vol. 48, No. 1, 2006, pp. 137-153.